Calcium aluminoferrite
# Calcium aluminoferrite

Calcium aluminoferrite (Ca $_2(Al,Fe)$ $_2O$ $_5)$ is a dark brown crystalline phase commonly found in cements. In the cement industry it is termed tetra-calcium aluminoferrite or ferrite. In cement chemist notation (CCN), it is abbreviated as C $_4AF$ meaning 4CaO·Al $_2O$ $_3·Fe$ $_2O$ $_3$ in the oxide notation. It also exists in nature as the rare mineral brownmillerite.

## Properties of the pure phase

In the absence of elements other than calcium, aluminium, iron and oxygen, calcium aluminoferrite forms a solid solution series of formula Ca $_2(Al$ $_xFe$ $_{1–x})$ $_2O$ $_5$ for all values of x in the range $0–0.7.^{:28–32}$ Compositions with x > 0.7 do not exist at ordinary pressures (see dicalcium aluminate). The crystal is orthorhombic, and is normally lath-like. Its density varies from 4026 $kg·m^{−3}$ (x = 0) to 3614 $kg⋅m^{−3}$ (x = 0.7). All compositions melt incongruently in the range 1400−1450 °C. They are ferromagnetic, progressively more so as iron content increases. These phases are easily prepared from the oxides.

## Phases in Portland cement clinker

In Portland cement clinker, calcium aluminoferrite (C $_4AF)$ occurs as an "interstitial phase", crystallizing from the melt as the reaction end-product of the flux components (Al $_2O$ $_3$ and Fe $_2O$ $_3)$ added in the raw materials to lower the high melting point of the oxide mix CaO-SiO $_2.$ Its presence in clinker is solely due to the need to obtain liquid at the peak kiln processing temperature (1400−1450 °C), facilitating the formation of the desired silicate phases. Apart from this benefit, its effects on cement properties are little more than those of a diluent. Its forms an impure solid solution that deviates markedly in composition from the simple chemical formula. The calcium aluminoferrite phase acts as a repository for many of the minor elements in the clinker. Most of the transition metals in the cement are found in the ferrite phase, notably titanium, manganese and zinc. There is also a substantial amount of magnesium and silicon, and because of this, oxides other than CaO, Al $_2O$ $_3$ and Fe $_2O$ $_3$ often make up 15% of the mass of the calcium aluminoferrite. This substitution reduces its melting point to around 1350 °C.

The typical chemical composition of calcium aluminoferrite (C $_4AF)$ for three different clinker bulk Fe $_2O$ $_3$ contents is given in the next $table.^{:10}^,^{:160}$ The calcium aluminoferrite mean composition is clearly dominated by CaO (43.7 wt. %), Al $_2O$ $_3$ (19.3 wt %), and Fe $_2O$ $_3$ (25.4 wt. %). The mean contents in SiO $_2$ (4.2 wt. %) and other oxides are marginal.

Chemical composition of calcium aluminoferrite (C $_4AF)$ as a function of the bulk concentration (mass %, or wt. %) of Fe $_2O$ $_3$ in the clinker :

| Oxide | Mass % | Mass % | Mass % |
| - | - | - | - |
| Bulk Fe $_2O$ $_3$ in clinker | 0.29 | 2.88 | 4.87 |
| SiO $_2$ | 4.0 | 2.6 | 6.1 |
| Al $_2O$ $_3$ | 20.2 | 20.8 | 17.0 |
| Fe $_2O$ $_3$ | 24.5 | 23.9 | 27.7 |
| CaO | 44.6 | 46.4 | 40.2 |
| MgO | 3.7 | 3.1 | 4.9 |
| Na $_2O$ | 0.1 | 0.1 | 0.1 |
| K $_2O$ | 0.1 | 0.1 | 0.1 |
| TiO $_2$ | 1.9 | 2.7 | 1.7 |
| Mn $_2O$ $_3$ | 0.1 | 0.3 | 1.5 |
| ZnO | 1.1 | 0.1 | 0.9 |

Note that the sum of Al $_2O$ $_3$ and Fe $_2O$ $_3$ contents in calcium aluminoferrite (C $_4AF)$ in the table here above remains constant at 44.7 mass % as illustrated in the table here below.

Sum of Al $_2O$ $_3$ and Fe $_2O$ $_3$ in C $_4AF$ in the above table :

| Oxide | Mass % | Mass % | Mass % |
| - | - | - | - |
| Bulk Fe $_2O$ $_3$ in clinker | 0.29 | 2.88 | 4.87 |
| Al $_2O$ $_3$ | 20.2 | 20.8 | 17.0 |
| Fe $_2O$ $_3$ | 24.5 | 23.9 | 27.7 |
| Sum | 44.7 | 44.7 | 44.7 |

## Behavior in cements

Calcium aluminoferrite (C $_4AF)$ has little effect upon the physical properties of cement. On hydration it $forms^{:175}$ hydrogarnet (4 CaO·Al $_2O$ $_3·$ n H $_2O)$ and hydrated iron oxide gel. In principle, this is a fast and energetic exothermic reaction, but precipitation of an insoluble layer of hydrated iron oxide upon the calcium aluminoferrite crystal surface forms a barrier to further reaction. In the case of Portland cement, subsequent slow reaction with dissolved sulfate forms AFm phases, which have negligible strength-giving properties. In the case of calcium aluminate cements $(CAC),^{:726}$ the situation is less clear-cut, but there is little contribution to early strength. Calcium aluminoferrite is also present in calcium sulfoaluminate (CSA) cements, and again contributes no strength.

